#------------------------------------------------------------------------------
#$Date: 2016-02-20 02:53:41 +0200 (Sat, 20 Feb 2016) $
#$Revision: 176768 $
#$URL: svn://www.crystallography.net/cod/cif/2/10/56/2105634.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/. The original data for this entry
# were provided by IUCr Journals, http://journals.iucr.org/.
#
# The file may be used within the scientific community so long as
# proper attribution is given to the journal article from which the
# data were obtained.
#
data_2105634
loop_
_publ_author_name
'Ehrenberg, H.'
'Hartmann, T.'
'Wltschek, G.'
'Fuess, H.'
'Morgenroth, W.'
'Krane, H.-G.'
_publ_section_title
;
 The crystal structure of Tm₅Re₂O₁₂
;
_journal_issue                   6
_journal_name_full               'Acta Crystallographica Section B'
_journal_page_first              849
_journal_page_last               852
_journal_paper_doi               10.1107/S0108768199005194
_journal_volume                  55
_journal_year                    1999
_chemical_formula_sum            'O12 Re2 Tm5'
_chemical_formula_weight         1409.05
_chemical_name_systematic        'Pentathulium dirhenium dodecaoxide'
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 107.816(2)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   12.3717(7)
_cell_length_b                   5.6744(3)
_cell_length_c                   7.4805(4)
_cell_measurement_reflns_used    460
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      38.89
_cell_measurement_theta_min      3.43
_cell_volume                     499.96(5)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full .717
_diffrn_measured_fraction_theta_max .717
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       omega-scans
_diffrn_radiation_monochromator  silicon
_diffrn_radiation_source         synchrotron
_diffrn_radiation_type           synchrotron
_diffrn_radiation_wavelength     .42750
_diffrn_reflns_av_R_equivalents  .0532
_diffrn_reflns_av_sigmaI/netI    .0912
_diffrn_reflns_limit_h_max       36
_diffrn_reflns_limit_h_min       -36
_diffrn_reflns_limit_k_max       16
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       20
_diffrn_reflns_limit_l_min       -21
_diffrn_reflns_number            8671
_diffrn_reflns_theta_full        38.89
_diffrn_reflns_theta_max         38.89
_diffrn_reflns_theta_min         3.43
_diffrn_standards_number         0
_exptl_absorpt_coefficient_mu    16.587
_exptl_absorpt_correction_T_max  .85
_exptl_absorpt_correction_T_min  .19
_exptl_absorpt_correction_type   empirical
_exptl_crystal_colour            black
_exptl_crystal_density_diffrn    9.360
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       needle
_exptl_crystal_F_000             1182
_refine_diff_density_max         14.225
_refine_diff_density_min         -12.324
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.246
_refine_ls_hydrogen_treatment    mixed
_refine_ls_matrix_type           full
_refine_ls_number_parameters     52
_refine_ls_number_reflns         4961
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.246
_refine_ls_R_factor_all          .0849
_refine_ls_R_factor_gt           .0682
_refine_ls_shift/su_max          .000
_refine_ls_shift/su_mean         .000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0103P)²+1.6684P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_ref         .1518
_reflns_number_gt                4165
_reflns_number_total             4961
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            os0018.cif
_cod_data_source_block           tm5
_cod_original_sg_symbol_H-M      'C 2/m'
_cod_database_code               2105634
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_calc_flag
_atom_site_refinement_flags
_atom_site_occupancy
_atom_site_type_symbol
Re1 .0000 .28367(4) .0000 .00224(3) Uani d S 1 Re
Tm1 .5000 .0000 .5000 .00381(5) Uani d S 1 Tm
Tm2 .31373(2) .5000 .17505(5) .00319(4) Uani d S 1 Tm
Tm3 .19638(2) .0000 .35973(5) .00313(4) Uani d S 1 Tm
O1 .0012(4) .0000 .1787(8) .0057(5) Uani d S 1 O
O2 .4989(5) .0000 .2053(9) .0076(6) Uani d S 1 O
O3 .3459(3) .2520(8) .4265(7) .0060(4) Uani d . 1 O
O4 .1655(3) .2461(8) .0833(8) .0063(4) Uani d . 1 O
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
Re Re -3.8260 3.0990 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Tm Tm -3.3990 2.2040 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
O O -.0070 .0020 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
_geom_angle
O4 Re1 O4 . 2 167.5(3)
O4 Re1 O2 . 3_455 94.3(2)
O4 Re1 O2 2 3_455 93.5(2)
O4 Re1 O2 . 7 93.5(2)
O4 Re1 O2 2 7 94.3(2)
O2 Re1 O2 3_455 7 102.9(2)
O4 Re1 O1 . 5 85.53(19)
O4 Re1 O1 2 5 84.84(19)
O2 Re1 O1 3_455 5 168.14(17)
O2 Re1 O1 7 5 88.96(17)
O4 Re1 O1 . . 84.84(19)
O4 Re1 O1 2 . 85.53(19)
O2 Re1 O1 3_455 . 88.96(17)
O2 Re1 O1 7 . 168.14(17)
O1 Re1 O1 5 . 79.2(2)
O4 Re1 Re1 . 5_565 96.25(13)
O4 Re1 Re1 2 5_565 96.25(13)
O2 Re1 Re1 3_455 5_565 51.44(12)
O2 Re1 Re1 7 5_565 51.44(12)
O1 Re1 Re1 5 5_565 140.40(12)
O1 Re1 Re1 . 5_565 140.40(12)
O4 Re1 Re1 . 5 83.75(13)
O4 Re1 Re1 2 5 83.75(13)
O2 Re1 Re1 3_455 5 128.56(12)
O2 Re1 Re1 7 5 128.56(12)
O1 Re1 Re1 5 5 39.60(12)
O1 Re1 Re1 . 5 39.60(12)
Re1 Re1 Re1 5_565 5 180.0
O4 Re1 Tm2 . 3_445 126.39(16)
O4 Re1 Tm2 2 3_445 45.83(16)
O2 Re1 Tm2 3_455 3_445 80.03(15)
O2 Re1 Tm2 7 3_445 139.98(17)
O1 Re1 Tm2 5 3_445 90.49(12)
O1 Re1 Tm2 . 3_445 42.18(12)
Re1 Re1 Tm2 5_565 3_445 118.387(5)
Re1 Re1 Tm2 5 3_445 61.613(5)
O4 Re1 Tm2 . 7 45.83(16)
O4 Re1 Tm2 2 7 126.39(16)
O2 Re1 Tm2 3_455 7 139.98(17)
O2 Re1 Tm2 7 7 80.03(15)
O1 Re1 Tm2 5 7 42.18(12)
O1 Re1 Tm2 . 7 90.48(12)
Re1 Re1 Tm2 5_565 7 118.387(5)
Re1 Re1 Tm2 5 7 61.613(5)
Tm2 Re1 Tm2 3_445 7 123.225(9)
O4 Re1 Tm3 . 5 128.26(15)
O4 Re1 Tm3 2 5 43.82(16)
O2 Re1 Tm3 3_455 5 137.15(17)
O2 Re1 Tm3 7 5 81.53(13)
O1 Re1 Tm3 5 5 43.18(12)
O1 Re1 Tm3 . 5 90.29(13)
Re1 Re1 Tm3 5_565 5 118.028(5)
Re1 Re1 Tm3 5 5 61.972(5)
Tm2 Re1 Tm3 3_445 5 71.175(9)
Tm2 Re1 Tm3 7 5 82.869(9)
O4 Re1 Tm3 . . 43.82(16)
O4 Re1 Tm3 2 . 128.26(15)
O2 Re1 Tm3 3_455 . 81.53(13)
O2 Re1 Tm3 7 . 137.15(17)
O1 Re1 Tm3 5 . 90.29(13)
O1 Re1 Tm3 . . 43.18(12)
Re1 Re1 Tm3 5_565 . 118.028(5)
Re1 Re1 Tm3 5 . 61.972(5)
Tm2 Re1 Tm3 3_445 . 82.869(9)
Tm2 Re1 Tm3 7 . 71.175(9)
Tm3 Re1 Tm3 5 . 123.944(9)
O2 Tm1 O2 . 5_656 179.9990(10)
O2 Tm1 O3 . . 90.57(18)
O2 Tm1 O3 5_656 . 89.43(18)
O2 Tm1 O3 . 6 90.57(18)
O2 Tm1 O3 5_656 6 89.43(18)
O3 Tm1 O3 . 6 76.4(2)
O2 Tm1 O3 . 2_656 89.43(18)
O2 Tm1 O3 5_656 2_656 90.57(18)
O3 Tm1 O3 . 2_656 103.6(2)
O3 Tm1 O3 6 2_656 180.00(14)
O2 Tm1 O3 . 5_656 89.43(18)
O2 Tm1 O3 5_656 5_656 90.57(18)
O3 Tm1 O3 . 5_656 180.0(2)
O3 Tm1 O3 6 5_656 103.6(2)
O3 Tm1 O3 2_656 5_656 76.4(2)
O2 Tm1 Tm3 . . 91.27(15)
O2 Tm1 Tm3 5_656 . 88.73(15)
O3 Tm1 Tm3 . . 38.22(11)
O3 Tm1 Tm3 6 . 38.22(11)
O3 Tm1 Tm3 2_656 . 141.78(11)
O3 Tm1 Tm3 5_656 . 141.78(11)
O2 Tm1 Tm3 . 5_656 88.73(15)
O2 Tm1 Tm3 5_656 5_656 91.27(15)
O3 Tm1 Tm3 . 5_656 141.78(11)
O3 Tm1 Tm3 6 5_656 141.78(11)
O3 Tm1 Tm3 2_656 5_656 38.22(11)
O3 Tm1 Tm3 5_656 5_656 38.22(11)
Tm3 Tm1 Tm3 . 5_656 180.0
O4 Tm2 O4 6_565 . 78.9(2)
O4 Tm2 O3 6_565 6_565 77.20(18)
O4 Tm2 O3 . 6_565 124.16(14)
O4 Tm2 O3 6_565 . 124.16(14)
O4 Tm2 O3 . . 77.20(18)
O3 Tm2 O3 6_565 . 76.1(2)
O4 Tm2 O1 6_565 3 136.01(13)
O4 Tm2 O1 . 3 136.01(13)
O3 Tm2 O1 6_565 3 93.96(15)
O3 Tm2 O1 . 3 93.96(15)
O4 Tm2 O4 6_565 7 113.09(9)
O4 Tm2 O4 . 7 70.80(19)
O3 Tm2 O4 6_565 7 164.26(15)
O3 Tm2 O4 . 7 105.28(16)
O1 Tm2 O4 3 7 70.33(15)
O4 Tm2 O4 6_565 4 70.80(19)
O4 Tm2 O4 . 4 113.09(9)
O3 Tm2 O4 6_565 4 105.28(16)
O3 Tm2 O4 . 4 164.26(15)
O1 Tm2 O4 3 4 70.33(15)
O4 Tm2 O4 7 4 69.1(2)
O4 Tm2 Re1 6_565 3 99.45(12)
O4 Tm2 Re1 . 3 140.21(15)
O3 Tm2 Re1 6_565 3 93.32(11)
O3 Tm2 Re1 . 3 130.07(10)
O1 Tm2 Re1 3 3 37.36(9)
O4 Tm2 Re1 7 3 73.67(10)
O4 Tm2 Re1 4 3 34.85(9)
O4 Tm2 Re1 6_565 7 140.21(15)
O4 Tm2 Re1 . 7 99.45(12)
O3 Tm2 Re1 6_565 7 130.07(10)
O3 Tm2 Re1 . 7 93.32(11)
O1 Tm2 Re1 3 7 37.36(9)
O4 Tm2 Re1 7 7 34.85(9)
O4 Tm2 Re1 4 7 73.67(10)
Re1 Tm2 Re1 3 7 56.774(9)
O4 Tm2 Tm3 6_565 7_556 91.66(15)
O4 Tm2 Tm3 . 7_556 91.66(15)
O3 Tm2 Tm3 6_565 7_556 40.18(12)
O3 Tm2 Tm3 . 7_556 40.18(12)
O1 Tm2 Tm3 3 7_556 109.12(15)
O4 Tm2 Tm3 7 7_556 145.12(12)
O4 Tm2 Tm3 4 7_556 145.12(12)
Re1 Tm2 Tm3 3 7_556 128.067(9)
Re1 Tm2 Tm3 7 7_556 128.067(9)
O4 Tm2 Tm3 6_565 1_565 40.63(14)
O4 Tm2 Tm3 . 1_565 103.31(12)
O3 Tm2 Tm3 6_565 1_565 36.66(11)
O3 Tm2 Tm3 . 1_565 99.01(12)
O1 Tm2 Tm3 3 1_565 120.67(6)
O4 Tm2 Tm3 7 1_565 152.69(11)
O4 Tm2 Tm3 4 1_565 90.32(11)
Re1 Tm2 Tm3 3 1_565 99.999(7)
Re1 Tm2 Tm3 7 1_565 156.003(9)
Tm3 Tm2 Tm3 7_556 1_565 59.118(7)
O4 Tm2 Tm3 6_565 . 103.31(12)
O4 Tm2 Tm3 . . 40.63(14)
O3 Tm2 Tm3 6_565 . 99.01(12)
O3 Tm2 Tm3 . . 36.66(11)
O1 Tm2 Tm3 3 . 120.67(6)
O4 Tm2 Tm3 7 . 90.32(11)
O4 Tm2 Tm3 4 . 152.69(11)
Re1 Tm2 Tm3 3 . 156.003(9)
Re1 Tm2 Tm3 7 . 99.999(7)
Tm3 Tm2 Tm3 7_556 . 59.118(7)
Tm3 Tm2 Tm3 1_565 . 102.187(13)
O3 Tm3 O3 . 6 78.1(2)
O3 Tm3 O3 . 7_556 78.77(17)
O3 Tm3 O3 6 7_556 125.04(8)
O3 Tm3 O3 . 4_546 125.04(8)
O3 Tm3 O3 6 4_546 78.77(17)
O3 Tm3 O3 7_556 4_546 75.2(2)
O3 Tm3 O1 . . 137.90(12)
O3 Tm3 O1 6 . 137.90(12)
O3 Tm3 O1 7_556 . 89.37(15)
O3 Tm3 O1 4_546 . 89.37(15)
O3 Tm3 O4 . 6 117.10(13)
O3 Tm3 O4 6 6 74.35(17)
O3 Tm3 O4 7_556 6 158.69(15)
O3 Tm3 O4 4_546 6 103.27(16)
O1 Tm3 O4 . 6 69.33(14)
O3 Tm3 O4 . . 74.35(17)
O3 Tm3 O4 6 . 117.10(13)
O3 Tm3 O4 7_556 . 103.27(16)
O3 Tm3 O4 4_546 . 158.69(15)
O1 Tm3 O4 . . 69.33(14)
O4 Tm3 O4 6 . 70.3(2)
O3 Tm3 Re1 . 5 143.46(13)
O3 Tm3 Re1 6 5 102.19(12)
O3 Tm3 Re1 7_556 5 125.06(10)
O3 Tm3 Re1 4_546 5 90.07(11)
O1 Tm3 Re1 . 5 36.93(9)
O4 Tm3 Re1 6 5 34.02(9)
O4 Tm3 Re1 . 5 73.26(11)
O3 Tm3 Re1 . . 102.19(12)
O3 Tm3 Re1 6 . 143.46(13)
O3 Tm3 Re1 7_556 . 90.07(11)
O3 Tm3 Re1 4_546 . 125.06(10)
O1 Tm3 Re1 . . 36.93(9)
O4 Tm3 Re1 6 . 73.26(11)
O4 Tm3 Re1 . . 34.02(9)
Re1 Tm3 Re1 5 . 56.055(9)
O3 Tm3 Tm2 . 7_556 93.18(13)
O3 Tm3 Tm2 6 7_556 93.18(13)
O3 Tm3 Tm2 7_556 7_556 39.71(12)
O3 Tm3 Tm2 4_546 7_556 39.71(12)
O1 Tm3 Tm2 . 7_556 103.06(14)
O4 Tm3 Tm2 6 7_556 142.98(11)
O4 Tm3 Tm2 . 7_556 142.98(11)
Re1 Tm3 Tm2 5 7_556 123.051(8)
Re1 Tm3 Tm2 . 7_556 123.051(8)
O3 Tm3 Tm3 . 7_556 39.78(12)
O3 Tm3 Tm3 6 7_556 104.03(11)
O3 Tm3 Tm3 7_556 7_556 39.00(10)
O3 Tm3 Tm3 4_546 7_556 101.62(12)
O1 Tm3 Tm3 . 7_556 117.96(6)
O4 Tm3 Tm3 6 7_556 154.15(11)
O4 Tm3 Tm3 . 7_556 88.67(11)
Re1 Tm3 Tm3 5 7_556 152.892(11)
Re1 Tm3 Tm3 . 7_556 97.833(8)
Tm2 Tm3 Tm3 7_556 7_556 62.211(11)
O3 Tm3 Tm3 . 7_546 104.03(11)
O3 Tm3 Tm3 6 7_546 39.78(12)
O3 Tm3 Tm3 7_556 7_546 101.62(12)
O3 Tm3 Tm3 4_546 7_546 39.00(10)
O1 Tm3 Tm3 . 7_546 117.96(6)
O4 Tm3 Tm3 6 7_546 88.67(11)
O4 Tm3 Tm3 . 7_546 154.15(11)
Re1 Tm3 Tm3 5 7_546 97.834(8)
Re1 Tm3 Tm3 . 7_546 152.892(11)
Tm2 Tm3 Tm3 7_556 7_546 62.211(11)
Tm3 Tm3 Tm3 7_556 7_546 106.672(17)
Re1 O1 Re1 5 . 100.8(2)
Re1 O1 Tm2 5 3_445 100.46(15)
Re1 O1 Tm2 . 3_445 100.46(15)
Re1 O1 Tm3 5 . 99.89(14)
Re1 O1 Tm3 . . 99.89(14)
Tm2 O1 Tm3 3_445 . 147.8(3)
Re1 O2 Re1 3_545 7 77.1(2)
Re1 O2 Tm1 3_545 . 141.43(12)
Re1 O2 Tm1 7 . 141.43(12)
Tm3 O3 Tm2 . . 106.39(18)
Tm3 O3 Tm3 . 7_556 101.23(17)
Tm2 O3 Tm3 . 7_556 100.12(16)
Tm3 O3 Tm1 . . 102.71(17)
Tm2 O3 Tm1 . . 120.0(2)
Tm3 O3 Tm1 7_556 . 123.9(2)
Re1 O4 Tm2 . . 134.1(2)
Re1 O4 Tm3 . . 102.2(2)
Tm2 O4 Tm3 . . 101.88(19)
Re1 O4 Tm2 . 7 99.3(2)
Tm2 O4 Tm2 . 7 109.20(19)
Tm3 O4 Tm2 . 7 108.40(17)
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_site_symmetry_2
_geom_bond_distance
Re1 O4 . 1.961(4)
Re1 O4 2 1.961(4)
Re1 O2 3_455 1.969(5)
Re1 O2 7 1.969(5)
Re1 O1 5 2.089(4)
Re1 O1 . 2.089(4)
Re1 Re1 5_565 2.4551(5)
Re1 Re1 5 3.2193(5)
Re1 Tm2 3_445 3.3857(3)
Re1 Tm2 7 3.3857(3)
Re1 Tm3 5 3.4255(3)
Re1 Tm3 . 3.4256(3)
Tm1 O2 . 2.201(6)
Tm1 O2 5_656 2.201(6)
Tm1 O3 . 2.311(4)
Tm1 O3 6 2.311(4)
Tm1 O3 2_656 2.311(4)
Tm1 O3 5_656 2.311(4)
Tm1 Tm3 . 3.5775(3)
Tm1 Tm3 5_656 3.5775(3)
Tm2 O4 6_565 2.267(4)
Tm2 O4 . 2.267(4)
Tm2 O3 6_565 2.285(5)
Tm2 O3 . 2.285(5)
Tm2 O1 3 2.312(4)
Tm2 O4 7 2.461(5)
Tm2 O4 4 2.461(5)
Tm2 Re1 3 3.3857(3)
Tm2 Re1 7 3.3857(3)
Tm2 Tm3 7_556 3.5204(6)
Tm2 Tm3 1_565 3.646(3)
Tm2 Tm3 . 3.646(3)
Tm3 O3 . 2.269(4)
Tm3 O3 6 2.269(4)
Tm3 O3 7_556 2.307(5)
Tm3 O3 4_546 2.307(5)
Tm3 O1 . 2.380(5)
Tm3 O4 6 2.426(5)
Tm3 O4 . 2.426(5)
Tm3 Re1 5 3.4256(3)
Tm3 Tm2 7_556 3.5204(6)
Tm3 Tm3 7_556 3.5370(4)
Tm3 Tm3 7_546 3.5370(4)
O1 Re1 5 2.089(4)
O1 Tm2 3_445 2.312(4)
O2 Re1 3_545 1.969(5)
O2 Re1 7 1.969(5)
O3 Tm3 7_556 2.307(5)
O4 Tm2 7 2.461(5)
